Nanostructuration of manganese oxides
by alkali cations towards higher activity in catalytic oxidation of soot and volatile organic compounds
under the guidance of prof. Andrzej Kotarba Materials and Surface Chemistry Group
Faculty of Chemistry Jagiellonian University
Papers I, II, VI, VII © Elsevier Paper III, V, VIII © Springer
Paper IV © Royal Society of Chemistry
I would like to thank:
Prof. Andrzej Kotarba for the many years of guidance, both scientific and personal, his commitment and patience.
Dr. Piotr Legutko, inż. for his tutelage, inspiration and friendship.
Dr. Wojciech Kaspera for the shared journey. Ook.
The Materials and Surface Chemistry Group for a place to develop and thrive.
Family and friends for their curiosity and support.
My wife, Basia Bazylewicz-Jakubek, for her immeasurable support and patience, especially during the preparation of this thesis.
The author of thesis was supported by the Polish National Science Centre project “Etiuda”
awarded by decision number UMO-2017/24/T/ST5/00413.
This thesis is a summary of the following Papers:
I. P. Legutko, T. Jakubek, W. Kaspera, P. Stelmachowski, Z. Sojka, A. Kotarba Soot oxidation over K-doped manganese and iron spinels - How potassium precursor nature and doping level change the catalyst activity
Catalysis Communications 43 (2014) 34-37
II. T. Jakubek, W. Kaspera, P. Legutko, P. Stelmachowski, A. Kotarba Surface versus bulk alkali promotion of cobalt-oxide catalyst in soot oxidation
Catalysis Communications 71 (2015) 37–41
III. T. Jakubek, W. Kaspera, P. Legutko, P. Stelmachowski, A. Kotarba How to Efficiently Promote Transition Metal Oxides by Alkali Towards Catalytic Soot Oxidation
Topics in Catalysis 59 (2016) 1083–1089
IV. P. Stelmachowski, P. Legutko, T. Jakubek, P. Indyka, Z. Sojka, L. Holmlid, A. Kotarba
Emission of highly excited electronic states of potassium from cryptomelane nanorods
Physical Chemistry Chemical Physics 17 (2015) 26289-26294 V. T. Jakubek, C. Hudy, J. Gryboś, H. Manyar, A. Kotarba
Thermal transformation of birnessite (OL) towards highly active cryptomelane (OMS-2) catalyst for soot oxidation
Catalysis Letters 149 (2019) 2218-2225
VI. T. Jakubek, C. Hudy, P. Indyka, E. Nowicka, S. Golunski, A. Kotarba Influence of different intra-layer alkali cations on the catalytic activity of birnessite in soot and VOCs oxidation
submitted to Applied Catalysis A
VII. T. Jakubek, C. Hudy, P. Indyka, E. Nowicka, S. Golunski, A. Kotarba
Effect on soot and VOC combustion activity of noble metal addition to alkali- exchanged cryptomelane-based catalysts
submitted to Catalysis Communications VIII. T. Jakubek, K. Ralphs, A. Kotarba, H. Manyar
Nanostructured Potassium-Manganese Oxides Decorated with Pd
Nanoparticles as Efficient Catalysts for Low-Temperature Soot Oxidation Catalysis Letters 149 (2018) 100-106
My contribution to the appended Papers
I. The synthesis, planning and performing of most of the experimental work (X-ray diffraction, Raman spectroscopy, work function and temperature programmed oxidation of soot measurements) concerning manganese-based catalysts, data analysis and interpretation as well as draft preparation and proofing
II. The synthesis, planning and performing of most of the experimental work (X-ray fluorescence, X-ray diffraction, Raman spectroscopy and temperature programmed oxidation measurements) concerning nanostructured catalysts, data analysis and interpretation as well as manuscript preparation and proofing
III. The synthesis, planning and performing of all of the experimental work (X-ray fluorescence, X-ray diffraction, Raman spectroscopy and temperature programmed oxidation measurements) concerning manganese-based and nanostructured catalysts, data analysis and interpretation as well as manuscript preparation and proofing
IV. The synthesis, planning and performing of all of the experimental work (excluding TEM), data analysis and interpretation as well as draft preparation and proofing
V. The planning of all and performance of part of the experimental work (X-ray diffraction, Raman spectroscopy, specific surface area), supervision over the remaining experimental work, data analysis and interpretation as well as manuscript preparation and proofing
VI. The planning of all and performance of part of the experimental work (specific surface area, temperature programmed oxidation of methane and propane), supervision over the remaining experimental work, data analysis and interpretation as well as manuscript preparation and proofing
VII. The synthesis, planning and performing of all of the experimental work (excluding TEM), data analysis and interpretation as well as manuscript preparation and proofing
VIII. The planning and performing of part of the experimental work (Raman spectroscopy, H2-temperature programmed reduction, temperature programmed oxidation of soot), data analysis and interpretation as well as manuscript preparation and proofing
The results found in this work were presented at the following conferences:
1. International Conference on Catalysis and Surface Chemistry 2. 8th World Congress on Oxidation Catalysis
3. 13th European Congress on Catalysis (Europacat XIII) 4. XI Copernican International Young Scientists Conference 5. XLIX Ogólnopolskie Kolokwium Katalityczne
6. 7th Asia-Pacific Congress on Catalysis (APCAT-7)
7. International Workshop on Functional Nanoporous Materials “FuNaM”
8. Zjazd Naukowego Polskiego Towarzystwa Chemicznego 9. 13th Pannonian International Symposium on Catalysis
10. International Conference on Electrochemical Energy Science and Technology (EEST2016)
11. The 16th International Congress on Catalysis
12. Designing New Heterogeneous Catalysts: Faraday Discussion 13. XLVIII Ogólnopolskie Kolokwium Katalityczne
14. Tenth International Congress on Catalysis and Automotive Pollution Control (CAPoC10)
15. COST Action CM1104 “Reducible Oxide Chemistry. Structure and Functions”.
16. XII European Congress on Catalysis ”Catalysis: Balancing the use of fossil and renewable resources” (EuropaCat XII)
17. 8. Kongres Technologii Chemicznej "Surowce - energia - materialy"
18. XLVII Ogólnopolskie Kolokwium Katalityczne
Additional Papers co-authored, which were not appended to this work:
1. P. Stelmachowski, P. Legutko, T. Jakubek, A. Kotarba, Phase evolution and electronic properties of cryptomelane nanorods, Journal of Alloys and Compounds 767 (2018) 592-599
2. P. Stelmachowski, A.H.A. Monteverde Videla, T. Jakubek, A. Kotarba, S. Specchia, The Effect of Fe, Co, and Ni Structural Promotion of Cryptomelane (KMn8O16) on the Catalytic Activity in Oxygen Evolution Reaction, Electrocatalysis 9(6) (2018), 762-769
3. P. Legutko, T. Jakubek, W. Kaspera, P. Stelmachowski, Z. Sojka, A. Kotarba, Strong Enhancement of deSoot Activity of Transition Metal Oxides by Alkali Doping: Additive Effects of Potassium and Nitric Oxide, Topics in Catalysis 60 (2017) 162–170
4. P. Stelmachowski, A. Kopacz, T. Jakubek, P. Indyka, J. Markowski, M.
Wojtasik, L. Ziemiaoski, W. Krasodomski, G. Żak, Z. Sojka, A. Kotarba, Insights into Structure, Morphology and Reactivity of the Iron Oxide Based Fuel Borne Catalysts, Topics in Catalysis 60 (2017) 367-373
5. P. Stelmachowski, P. Legutko, A. Kopacz, T. Jakubek, P. Indyka, P. Pietrzyk, M. Wojtasik, J. Markowski, W. Krasodomski, L. Ziemiaoski, G. Żak, Z. Sojka, A. Kotarba, Role of chain length of the capping agents of iron oxide based fuel borne catalysts in the enhancement of soot combustion activity, Applied Catalysis B: Environmental 199 (2016) 489-493
6. A. L. Miller, M. Bowker, …, T. Jakubek, A. Corma, M. Claeys, H. Svengren, C. Friend, D. Lennon, J. Makepeace, H. Hunter, H. Manyar, Application of novel catalysts: general discussion, Faraday Discussions 188 (2016) 399-426 7. P. Selvam, J. Sauer, …, T. Jakubek, D. Willock, M. Craven, K. Sethu, R. Catlow,
R. Madix, H. Manyar, C. Friend, A. Corma, P. Wells, W. Ueda, A. Trunschke R. Palmer, Designing new catalysts: synthesis of new active structures:
general discussion, Faraday Discussions 188 (2016) 131-159
8. P. Legutko, W. Kaspera, T. Jakubek, P. Stelmachowski, A. Kotarba, Influence of Potassium and NO Addition on Catalytic Activity in Soot Combustion and Surface Properties of Iron and Manganese Spinels, Topics in Catalysis 56 (2013) 745
Głównym celem pracy doktorskiej było opracowanie katalizatora do niskotemperaturowego spalania sadzy oraz lotnych związków organicznych o efektywności działania konkurującej z obecnie stosowanymi układami komercyjnymi. Hipoteza badawcza sprawdzana w ramach projektu doktorskiego, opierała się na koncepcji, iż poprzez zaproponowane modyfikacje strukturalne (nanostrukturyzacja jonami metali alkalicznych) i powierzchniowe (dekoracja nanocząstkami metali szlachetnych) tlenków manganu można w znaczący sposób zoptymalizowad najistotniejsze parametry użytkowe katalizatora. W szczególności koncentrowano się na zmianach: właściwości elektrodonorowych (aktywacja tlenu na drodze transferu elektronu), mobilności tlenu sieciowego (ułatwienie działania mechanizmu Marsa-van Krevelena) oraz stabilności termicznej (zapewnienie wysokiej aktywności w czasie). Opracowanie docelowego układu katalitycznego realizowano w następujących etapach:
I. Określenie zmian strukturalnych pod wpływem wprowadzenia jonów potasu do struktury tlenku manganu (nanostrukturyzacja),
II. Określenie wpływu poszczególnych kationów grupy I (A = H+, Li+, Na+, K+, Rb+ oraz Cs+) na właściwości katalityczne birnesytu (AMn4O8) oraz kryptomelanu (AMn8O16) w reakcjach utleniania sadzy oraz lotnych związków organicznych (metan, propan),
III. Funkcjonalizacja nanocząstkami metali szlachetnych (Ag, Au, Pt, Pd) nanostrukturalnych faz tlenków mieszanych (K-Mn-O) w celu rozszerzenia ich aktywności katalitycznej na utlenianie lotnych związków organicznych.
Do charakterystyki przygotowanych układów katalitycznych wykorzystano szeroki wachlarz metod eksperymentalnych: do określenia składu pierwiastkowego (XRF, XPS), fazowego (XRD, RS), morfologii (SEM, TEM), powierzchni (N2-BET, XPS), oraz stabilności termicznej i aktywności w spalaniu sadzy i lotnych związków organicznych (TPR, TGA/DTA, TPO). Istotnym dla określenia mechanizmów reakcji utleniania były badania właściwości elektrodonorowych powierzchni (pomiary pracy wyjścia metodą Kelvina) oraz termicznej desorpcji potasu (SR-TAD).
Początkowe badania dotyczące modyfikacji struktury tlenku manganu alkaliami wykazały, że tworzenie nanostrukturyzowanych faz zwiększa aktywnośd katalityczną w procesie dopalania sadzy. Otrzymane fazy o strukturze warstwowej (birnesyt) oraz tunelowej (kryptomelan) zawdzięczają swoją wysoką aktywnośd ukierunkowanej mobilności potasu (desorpcja kierunkowana warstwami
lub tunelami, możliwośd desorpcji w wysokoenergetycznych formach atomów Rydberga), korzystnej morfologii (nanopręty kryptomelanu) oraz zwiększonej aktywności manganowych centrów redoksowych (wykorzystanie tlenu sieciowego w mechanizmie Marsa-van Krevelena). Korzystny efekt promocji potasem wykazano zarówno dla promocji powierzchniowej, jak i strukturalnej [Publikacje I, II, III]. Publikację IV poświęcono zbadaniu efektu desorpcji potasu z powierzchni kryptomelanu, wykazująd desorpcję zarówno w formie atomowej, jonowej jak również wysokoenergetycznych stanów Rydberga.
Publikacja V dotyczyła termicznej transformacji birnesytu do kryptomelanu, powodując powstanie fazy o większej aktywności w luźnym kontakcie z sadzą.
Jak wykazano w publikacjach VI oraz VII wprowadzenie różnych kationów I grupy ma znaczący wpływ na strukturę birnesytu oraz kryptomelanu. Wprowadzenie poszczególnych kationów grupy I do tunelowej struktury kryptomelanu powodowało obniżenie zarówno pracy wyjścia, jak i temperatury spalania sadzy.
Pozwoliło to na określenie mechanizmu inicjacji reakcji spalania, jako aktywacji tlenu na drodze transferu elektronu z powierzchni katalizatora [Publikacja VI].
Dla birnesytu, wprowadzenie kationów grupy I również powodowało obniżenie pracy wyjścia zgodnie z szeregiem energii jonizacji, jednak korelacja pracy wyjścia z aktywnością katalityczną była w tym przypadku odwrócona. Dla serii birnesytowej aktywnośd katalityczną powiązano bezpośrednio z ilością tlenu sieciowego desorbującego z materiału w oknie temperaturowym reakcji (mechanizm Marsa- van Krevelena) [Publikacja VII]. Stwierdzono, że promocja powierzchniowa nanocząstkami platyny znacząco poprawia aktywnośd w reakcjach dopalania lotnych związków organicznych *Publikacja VII], podczas gdy wprowadzenie nanocząstek srebra oraz palladu poprawia aktywnośd w dopalaniu sadzy [Publikacje VI - VIII].
Kompleksowe badania wykonane podczas pracy doktorskiej pozwoliły na ustalenie różnych mechanizmów utleniania sadzy oraz lotnych związków organicznych dla birnesytu oraz kryptomelanu. Otrzymane wyniki wskazały możliwości funkcjonalizacji tlenków manganu w kierunku wysokiej aktywności katalitycznej poprzez nanostrukturyzacje alkaliami (wzrost aktywności w dopalaniu sadzy) oraz dekoracje nanocząstkami metali szlachetnych (wzrost aktywności w dopalaniu lotnych związków organicznych). Najaktywniejsze układy pozwoliły na obniżenie temperatury spalania sadzy o 300°C (Ag/KMn8O16, Pd/KMn4O8) oraz lotnych związków organicznych (CH4 i C3H8) w 350 - 400°C (Pt/KMn8O16).
The main aim of the doctoral thesis was to design a catalyst for the low- temperature combustion of soot and volatile organic compounds with efficiency competing with the currently used commercial systems. The research hypothesis tested in this work was based on the idea, that through the proposed structural (nanostructuration with alkali metal ions) and surface (decoration with noble metal nanoparticles) modifications of manganese oxides, the most important parameters for catalyst performance can be significantly optimized. In particular, the main focus was on the changes in electrodonor properties (activation of oxygen through electron transfer), lattice oxygen mobility (facilitation of the Mars-van Krevelen mechanism) as well as thermal stability (ensuring high activity over time).
The development of the target catalytic system was carried out in the following stages:
I. Determination of structural changes caused by the introduction of potassium ions into the manganese oxide structure (nanostructuration), II. Determination of the discrete influence of group I cations (A = H+, Li+, Na+,
K+, Rb+ and Cs+) on the catalytic properties of birnessite (AMn4O8) and cryptomelane (AMn8O16) in the reactions of soot and volatile organic compound (methane, propane) oxidation,
III. Functionalization with precious metal nanoparticles (Ag, Au, Pt, Pd) of mixed-oxide nanostructured phases (K-Mn-O) to extend their catalytic activity in volatile organic compound oxidation.
A wide range of experimental methods were used to characterize the prepared catalytic systems: to determine the elemental composition (XRF, XPS), phase (XRD, RS), morphology (SEM, TEM), surface (N2-BET, XPS), thermal stability and activity in soot and volatile organic compound oxidation (TPR, TGA/DTA and TPO). An important factor in determining the mechanisms of the oxidation reactions were the investigations of electrodonor properties of the catalyst surface (work function through the Kelvin method) as well as the thermal desorption of potassium (SR-TAD).
Initial studies on the modification of the structure of manganese oxides with alkali showed that the formation of nanostructured phases increases catalytic activity in soot combustion. The prepared layered (birnessite) and tunnelled (cryptomelane) structures owe their high activity to the directed potassium mobility (desorption directed by layers or tunnels, the possibility of high energy
Rydberg atom desorption), favourable morphology (cryptomelane nanorods) and the increased activity of manganese redox centers (use of lattice oxygen in the Mars-van Krevelen mechanism). The beneficial effect of potassium promotion was demonstrated for both surface and structural promotion [Papers I, II, III]. The fourth Paper is devoted to investigating the effect of potassium desorption from the surface of cryptomelane, showing desorption in both atomic and ionic potassium forms as well as the high energy Rydberg species.
The topic of Paper V was the thermal transformation of birnessite to cryptomelane, resulting in a phase with greater activity in loose contact with soot. As shown in Papers VI and VII, the introduction of different group I cations has a significant effect on the structure of birnessite and cryptomelane. The introduction of individual group I cations into the tunnel structure of cryptomelane cause a decrease in both the work function and the temperature of soot combustion.
The results established the electron transfer from catalyst surface to oxygen as the first step in the oxidation mechanism over cryptomelane-based catalysts [Paper VI].
For birnessite, the introduction of group I cations also resulted in a decrease of work function in accordance with the lowering ionization energies of the group, however, the correlation of the work function with catalytic activity was in this case reversed. For the birnessite series, the catalytic activity was directly related to the amount of lattice oxygen desorbing from the material in the temperature window of the reaction (Mars-van Krevelen mechanism) [Paper VII] It was found, that surface promotion with platinum nanoparticles significantly improves the catalytic activity during volatile organic compound oxidation [Paper VII], while the introduction of silver and palladium nanoparticles improve the activity in soot combustion [Papers VI-VIII].
The comprehensive research carried out during the doctoral thesis allowed for the establishment of the various mechanisms for the oxidation of soot and volatile organic compounds over birnessite and cryptomelane. The obtained results indicated the possibility to functionalize manganese oxides towards high catalytic activity through alkaline nanostructuration (increased activity in soot combustion) and decoration with noble metal nanoparticles (increase of activity in volatile organic compound combustion). The most active systems allowed the lowering of the temperature of soot combustion by 300°C (Ag/KMn8O16, Pd/KMn4O8) and volatile organic compounds (CH4 and C3H8) by 350 – 400°C (Pt/KMn8O16).
The following work, titled “Nanostructuration of manganese oxides by alkali cations towards higher activity in catalytic oxidation of soot and volatile organic compounds” was conducted in the Materials and Surface Chemistry Group at the Faculty
of Chemistry of the Jagiellonian University. The author was supported by the Polish National Science Centre project “Etiuda” awarded by decision number UMO-2017/24/T/ST5/00413, which made it possible to perform part of the studies abroad at the Cardiff Catalysis Institute in Cardiff, Wales.
The results of the research conducted during the course of the work was presented in the form of 8 Papers in reputable journals (such as: Topics in Catalysis, Catalysis Communications, Physical Chemistry Chemical Physics and Catalysis Letters) as well as during several national and international conferences in both oral and poster forms.
The work has been divided into 3 sections: introduction (a review of the current state-of-the-art, motivation), an experimental section (strategy of investigation and description of used methods), which is followed by the results and discussion of the presented 8 Papers comprising the thesis. The work concludes with a summary of the most important points determined during the course of the work.
Table of contents
1. Introduction ... 1
1.1.Combustion of fuels ... 1
1.2.Volatile organic compounds ... 1
1.3.Soot ... 3
1.4.Methods of pollutant elimination ... 5
1.5.Components of soot and VOC combustion catalysts ... 8
Supports ... 8
Active phases ... 9
Promoters ... 10
2. Motivation ... 13
3. Strategy of investigation ... 15
3.1.Soot and volatile organic compounds ... 15
3.2.Birnessite ... 16
3.3.Cryptomelane ... 17
3.4.Aim and research strategy ... 18
4. Experimental Methods... 20
4.1.Elemental composition... 21
X-ray Fluorescence Spectroscopy (XRF) ... 21
4.2.Phase composition ... 21
X-ray Diffraction (XRD) ... 21
Raman Spectroscopy (RS) ... 22
4.3.Morphological characterization ... 22
Scanning Electron Microscopy (SEM) ... 22
Transmission Electron Microscopy (TEM) ... 23
4.4.Surface characterization... 23
N2-BET specific surface area analysis (BET) ... 23
X-ray Photoelectron Spectroscopy (XPS) ... 23
Measuring work function using the Kelvin method (WF) ... 24
Species Resolved-Thermal Alkali Desorption (SR-TAD) ... 25
4.5.Catalytic activity and stability ... 26
Temperature-Programmed Reduction (TPR) ... 26
Thermogravimetric Analysis/Differential Thermal Analysis (TGA/DTA) ... 26
Temperature-Programmed Oxidation (TPO) ... 27
5. Results and discussion ... 29
5.1.Initial state-of-the-art ... 30
5.2.List of investigated materials ... 30
5.3.Nanostructuration ... 32
Investigating the nanostructuration process ... 32
Effects of nanostructuration on the pro-catalytic properties ... 35
5.4.Effect of intercalated alkali cation ... 39
Cryptomelane ... 39
Birnessite ... 42
5.5.Decoration of birnessite and cryptomelane with noble metal nanoparticles ... 46
Effect on properties... 47
Effect on soot and VOC oxidation ... 49
6. Recapitulation ... 56
7. Conclusions ... 59
Nanostructuration ... 59
Effect of intercalated cation ... 59
Decoration of K-Mn-O nanostructures with noble metal nanoparticles ... 59
8. References ... 61
Appended Paper ... 68
1.1. Combustion of fuels
All life on Earth exists in a perpetual struggle to gather and sustain the necessary energy to continue living and to produce offspring. For humans, civilization has progressed enough to not only provide the necessary energy to sustain us and provide for our families, but also to allow us to live on a higher level of comfort.
With this, our energy requirements increase substantially and must be produced from many different sources. These can range from harnessing renewable or long- lasting sources of energy (nuclear wind, water, geothermal) to the more finite such as fossil fuels. Energy is extracted from fossil fuels through their combustion, where the energy from the oxidation reaction is transformed into mechanical energy.
On a small scale, this process occurs in combustion engines, which play a crucial role in the transportation sector. The imperfect design and ever-changing conditions found in engines means that typically pyrolysis or incomplete combustion of the carbon-containing fuels ubiquitously take place, leading to the formation and emission of cancerogenic and mutagenic products of these reactions. Among these products soot and volatile organic compounds (VOC’s) are among the most dangerous.
1.2. Volatile organic compounds
Volatile organic compounds (VOCs), which can be described as “any compound of carbon, excluding carbon monoxide, carbon dioxide, carbonic acid, metal carbides and ammonium carbonates which participates in atmospheric photochemical reactions” 1. Under this definition many different organic molecules can be treated as VOC’s, typically displaying high vapour pressure and low water solubility. VOCs are the precursors of ozone, photochemical smog and can also be highly harmful to human beings due to their toxic, malodorous, cancerogenic and mutagenic nature.
VOCs can escape into the environment due to a number of human activities such as transportation, industrial processes including power plants, gas stations, printing, shoemaking, chemical and pharmaceutical plants, petroleum refineries, automobile manufacturers, food processors, furniture/textile manufacturers, electronic component plants and vehicle exhaust 2. In the transportation sector, combustion engines are the source of VOC emissions produced during the combustion of fuels such as diesel or gasoline (Fig. 1) 3. The reduction of these
2 emissions can be through the application of biofuels or through the application of exhaust gas aftertreatment.
Fig. 1 Diagram of pollutant emissions originating from the combustion of carbon fuels in vehicle engines
Due to their harmful nature and multiple sources, the emissions of VOC are controlled by legislation, with many countries agreeing to reduce the concentrations released into the environment. Catalytic systems are typically used in order to limit the escape of VOCs into the environment. Noble metal based catalysts are the main choice, due to their high activity, resistance to deactivation and ability to regenerate 4. Transition metal oxides are also being considered for these reactions, with cobalt and manganese oxides showing good activity but lower reaction rates than their noble metal based counterparts 1,5. Among the most common and toxic non-halogenated compounds a number are worth mentioning: formaldehyde, benzene, benzopyrene, toluene, propylene, phenol, acetone, styrene 6,7. A number of single and multiple aromatic compounds (polyaromatic hydrocarbons PAH) are also known to be highly toxic 6–8.
When VOC’s are present during oxidation reactions of fossil fuels, or are the fuels themselves, they may either escape into the environment or take part in the reaction. The optimum result is that of complete combustion to inert products such as CO2 and H2O. An alternative is the VOC is partially oxidized to an undesired by-product, which can also be a VOC. The VOC’s may also recombine with the surrounding fuel or other VOC’s to create new long chained hydrocarbons or aromatic structures. The latter typically form polycyclic particles, which can be thought of as graphene plates, which are known to orientate themselves randomly amongst themselves, becoming nucleation centers for further growth and further agglomeration of particles. The final result of this process are large particles of soot, which are equally dangerous.
Soot is formed in conditions characterized by high temperatures and low concentrations of oxygen, which favour the decomposition of carbon fuels instead of total oxidation. The formation process begins when remnants of the unburned fuel bond together to produce larger molecules, such as aromatic or polycyclic hydrocarbons (Fig. 2). These continue to polymerize, grow and coalesce into large, nanometric soot particles 9. In the inhomogeneous conditions present in reactors or engines the decomposition of fuels may occur through many different reaction pathways, forming many different half-products, which in the following stages of the reaction can lead to the condensation of soot. Therefore, soot composition can vary greatly, with the main components being typically amorphic carbon, graphite, fullerenes and many aliphatic and aromatic hydrocarbons. Upon emission into the environment, the nanometric size of soot particles allow them to become permanently suspended in the air, contributing to the formation of smog.
The suspended particles can also enter into living organisms, easily passing into our bodies through the respiratory system or even through skin, leading to a number of illnesses and cancero- or mutagenic changes. Long term exposure to soot particles can cause or potentiate many conditions, typically of the heart and lungs. The smallest soot particles also have the ability to modify DNA, causing mutations and cancerous changes.
4 Fig. 2 Soot formation reaction pathway
Numerous scientific studies have confirmed the threat soot poses to living organisms and the environment 10–15. It is estimated, that in Europe in 2018 nearly 422 000 premature deaths occurred due to exposure to particulate matter (which is substantially comprised of soot) with a size of 2.5 nm or less (PM2.5), with 44 500 of these deaths occurring in Poland 16. The suspended particles reduce air clarity, influence rainfall, accelerate the deterioration of monuments and disrupt ecosystems, lowering the speed with which plants and animals grow. Furthermore, when soot particles settle on ice or snow, the increased absorbance of sunlight increases the rate of melting, influencing global climate change 17. For Poland air pollution is a serious issues, as it regularly exceeds the norms of permitted concentrations of PM10 and PM2.5 18
5 The main anthropogenic sources of soot can be divided into stationary and mobile sources (Fig. 3). The most common stationary sources include coal power plants, waste incineration and households 19. Due to intense scrutiny and the tightening of regulations the first two sources can be easily controlled and monitored to keep the emission of soot to a minimum. The control of emission from household is more complicated. Here soot originates from heating furnaces, which can be fuelled by low-quality coal or, in the worst case, plastics and waste.
Monitoring is highly impeded in households, where the emission of soot particles is mainly mitigated through the exchange of old and inefficient furnaces for newer installations using gas or electricity, or by connecting the installation to the urban heating and power network.
Fig. 3 Depiction of the anthropogenic sources of soot together with their contribution to environmental pollution
The mobile sources consist mainly of vehicles, planes and ships powered by carbon fuels, which in their vast numbers leads to the production of large quantities of soot. Here, the changing conditions in the engines, the quality of the fuel and the design of the engine are crucial to the complete combustion of the used fuel.
Despite pressure from governments and the general populace, no suitable methods for both effective and inexpensive reduction of soot emissions to the environment have been found, although several technologies are presently used 20.
1.4. Methods of pollutant elimination
For both soot and VOCs produced in combustion engines many technologies have been developed to mitigate their emission into the environment. They are similar in their aim: the combustion of the pollutants to less dangerous products.
6 This is usually achieved through some form of thermal or catalytic combustion.
Some pre-reaction technologies include modifying the engine itself to be more optimized to the necessary conditions to aid in the total oxidation of the fuel.
Likewise, the fuel may also be modified with additives or exchanged for alternatives (such as alcohol or natural gas). The most effective thus far are post- reaction technologies based heavily on the use of catalysts to lower the reaction temperature, which include fuel borne catalysts (FBC), continuously regenerating traps (CRT) and diesel or gasoline particulate filters. The addition of catalyst precursors to the fuel stream is the basis of the FBC technology. In it, the catalyst is created in-situ during the combustion reaction. The added precursor is oxidized to a nanoparticle, which soot particles can build on and around. This enables high catalyst-soot contact and lowers the combustion temperature effectively. The CRT technology uses catalysts to oxidize NO present in the gas stream to NO2, which is a more effective oxidant and initiates the combustion process in lower temperature (even reaching ~250°C). This method is hindered by the quality of fuel, the engine function/temperature and the presence of NO.
Fig. 4 Methods of soot elimination. A) FBC - soot elimination due to increased soot-catalyst contact. B) CRT - soot combustion through oxidation of NO to NO2, which initiates soot oxidation. C) DPF - soot is accumulated on filter coated with catalyst lowering temperature of soot oxidation
7 The final technology makes use of particulate filters (Diesel Particulate Filter – DPF, Gasoline Particulate Filter – GPF). The filter walls are permeable to gases but not to solid fractions, which can lower particulate matter emissions by up to 99%. Every second channel in the filter is typically open at the source of the gas stream and blocked on the far side, with the remaining channels plugged the opposite way (plugged at the source and open at the exit). This forces the gas to pass through the porous walls, leaving the soot and other products of the combustion process behind. The soot is accumulated on the filter and burned either continuously or periodically in order to reduce the pressure drop and to increase the ability of the filter to trap additional pollutants. This process is known as regeneration. In order to burn the trapped soot a temperature of 600°C is required, which is not possible during normal engine operation. The filters must therefore be made from thermally stable materials. To artificially increase the exhaust gas temperature fuel can be injected in a delayed manner into the combustion chamber (post-injection) or behind the engine, causing a rise in temperature needed for the captured soot to combust. This type of regeneration is called active regeneration, whereas that occurring during normal engine function is called passive regeneration.
In order to lower the temperature, at which the adsorbed pollutant cake is combusted, catalytically active phases may be applied. First, a washcoat is applied to increase the surface area and act as a support for the active phases, which are then spread evenly over the surface of the washcoat.
Upon contact with the pollutants, the active phase in tandem with the support lowers the temperature of their combustion. In the case of soot, the contact between the active phase and the soot particle is important. Volatile pollutants on the other hand come into contact with the catalyst through adsorption on the catalyst surface, while passing through the filter walls or are combusted by active oxygen species formed over the active phases. The applied catalyst typically is also active in NO oxidation, combining the beneficial effects of both the FBC and CRT catalytic methods. The properties of the active phase may further be modified by decoration with promoters, further increasing the desired properties.
The components of soot and VOC combustion catalytic systems, comprised of the monolithic body, washcoat, active phases and promoters (Fig. 5), will be addressed in the following chapters.
8 Fig. 5 Diagram depicting the construction of a Diesel particulate filter
1.5. Components of soot and VOC combustion catalystsSupports
The supports for the typically used catalytic traps can be divided into 3 main groups: foams, fibre filters and wall-flow filters. The first and second support system is not considered efficient due to the deep filtration mechanism that they enable. This means not only the surface of the support filters the passing stream but also the pores. These systems are typically made of zirconia-toughened- alumina or – mullite (foams) or doped-alumina (fibre filters). Wall-flow filters are very efficient, capturing more than 90% of the traversing particles.
These supports make use of the alternatingly plugged channels and flow-through porous walls, as described above, in order to filter out the solid fraction from the exhaust stream. The support is typically comprised of partially sintered silica carbide (SiC) or cordierite (2MgO·2Al2O3·5SiO2) 21,22.
Ceria based catalysts are one of the most investigated supports for pollutant combustion as CeO2 alone, or in conjunction with other metals or metal oxides, exhibits high activity in soot and VOC oxidation. This is due to its excellent oxygen- buffering capacity and the high redox capabilities of the oxide. Numerous studies involve the addition of zirconium, rare earth elements and other metal/metal
9 oxides to the ceria framework in order to improve the oxygen storage capacity and redox properties of CeO2 23. There are also multiple accounts of modifying catalytic activity by controlling the morphology and specific surface area of the oxide.
Active phases Noble metals
Noble metal-based systems remain some of the most active and stable systems developed to date. The active phases of these systems are comprised of nanoparticles of platinum, palladium, rhodium as well as gold and silver. Despite their high cost and limited availability, noble metal-based systems are still intensely investigated.
The high activity of noble metal-based systems stems from their ability to oxidize NO to NO2, the oxidation properties of which greatly exceed that of O2, and due to the spillover mechanism, which the noble metal particles facilitate, during which active oxygen species formed over the catalyst are transferred to the pollutant and take part in the oxidation reaction. In order to increase the activity of the noble metals while keeping a small loading (and therefore lower price) the nanoparticles are dispersed evenly over a support. Investigations concern the preparation of small nanoparticles (maximizing surface area of the noble metal to its weight loading), even dispersion and metal-support interaction. The highest activities have been achieved on non-basic oxide supports, such as: SiO2, TiO2 or Ta2O524
Platinum is one of the most commonly investigated rare metals, especially when dispersed over a CeO2 support. The high surface area and high oxygen mobility of the cerium oxide aided by the high activity of Pt to oxidize NO to NO2 as well as enable the oxygen spillover effect makes the Pt/CeO2 catalyst extremely active in oxidation reactions, mainly through the Mars van Krevelen mechanism.
The advent of nanoparticle science has also revealed gold and silver as highly active catalysts. Gold was long thought to be inert, as large particles of gold do not show interesting catalytic properties, but preparing nanoparticles of the metal reveals the high activity in oxidation reactions, specifically in the oxidation of NO to NO2 25.
Transition Metal Oxides
An alternative to the expensive noble metal-based catalysts are transition metals oxides, which due to their high activity, abundance and low cost, form the largest group of investigated and applied non-noble metal based active phases.
For both soot and VOC oxidation similar systems are investigated, beginning from simple oxides (CeO2, ZnO2, TiO2, Fe2O3, NiO, CuO, Cr2O3, V2O5 and MoO3) 26–31,
10 mixed oxides (LiCoO2, CeO2-La2O3, Co3O4-CeO2, NiO-CeO2, TiO2-SiO2, NiCo2O4, Fe and CrCeO2) 29,32–37, perovskites 38–43, spinels 44–48 as well as complex mixed oxides (Sr0.8K0.2Ti0.9Cu0.1O3, Ce0.65Hf0.25M0.1O2−δ, (M = Tb, Sm, Nd, Pr, La), Co3O4 on TiO2
nanorods, Co3−xMnxAlOy, CuCexZr1−xOy/ZSM-5) 49–52. Numerous studies also show, that the activity of transition metal oxide based catalytic systems can be increased by dispersing noble metal nanoparticles on the surface of the active phase 25,53–57.
Among the transition metals oxides, manganese oxides have been the center of numerous scientific studies due to their interesting properties and high catalytic activities. Manganese based compounds are typically characterized as being inexpensive, abundant, environmentally friendly. Their curious properties have led to research and potential applications in diverse areas, including rechargeable lithium ion batteries, molecular adsorption, gas sensors, energy storage and magnetics 58–61. In catalysis, manganese oxides have also been evaluated as catalysts for several reactions, including C-H activation, cyclization, (de)hydrogenation and hydrosilylation 62–66. Furthermore, manganese oxides have been vigorously studied in oxidation reactions, including the oxidation of both soot and VOC 48,67–69. There high activity in oxidation reactions stems from the ease with which manganese can change its oxidation state, commonly ranging from +2 to +7 and due to the availability of facile lattice oxygen 63,68,70,71
An alternative way to increase the activity of active phases is through the use of alkali promoters. Studies show most alkali promotion is beneficial, though the best cost/activity ratio is typically found upon potassium promotion. For soot combustion, alkali promotion is shown to be highly beneficial, though numerous reaction mechanisms have been proposed to account for their action. These include: formation of compounds with low melting points (increases the catalyst- soot contact), the modification of the catalyst work function (activation of gas phase oxygen through electron transfer), mobility of alkali to the soot particles (destabilization of the hydrocarbons) or through incorporation of the alkali into the bulk of the material (synthesis of new, highly active phases). Which mechanism is prevalent depends on the alkali, the support as well as the method of promotion – surface or bulk.
11 Surface vs. bulk alkali location
The easiest way to promote a catalyst with alkali is through surface promotion.
The alkali is typically delivered through impregnation with a solution containing a precursor (usually a carbonate, less often nitrate or chloride) of the alkali, which decomposes during calcination. The aim is the even dispersion of the alkali on the surface of the material, not modifying the structure/morphology but only the properties of the surface. Therefore, surface promotion makes use mainly of the first 3 aforementioned mechanisms. The reaction between alkali and NOx found in the gas stream can lead to the formation of low melting point compounds such as KNO3 (melting temperature of KNO3 = 334°C) 72. Work function can be controlled by dispersing an appropriate amount of alkali on the catalyst surface, typically lowering work function until a certain coverage is attained 73. At higher temperatures, alkali atoms or ions can become highly mobile and can be transferred to the soot particle, where the alkali can lead to the deformation and destabilization of the soot components, leading to their facile combustion.
Additionally, it was proposed that excited states of alkali, known as Rydberg matter, can be responsible for the high activity of alkali containing catalysts by initiating the oxidation reactions due to the energy transfer from highly excited electrons.
Fig. 6 Schematic showing the effects of surface promotion (no structural change) versus bulk promotion
12 The second type of promotion, bulk promotion, occurs when the alkali enter into the structure of the active phase and modify it in a process called nanostructuration. This term is applied to materials, which were transformed to contain structures, which have a dimension in the nanoscale. In the case of birnessite and cryptomelane new structures are formed to accommodate the alkali, such as layers or tunnels, in which we find the alkali cations stabilized by the surrounding active phase. This process occurs in materials which can easily change their oxidation state, as the positive charge of the alkali cations must be neutralized by a negative charge in the materials matrix. This can increase the catalytic activity modified phase compared to the parent material due to the modification of the redox properties of the material. Furthermore, all the mechanisms are available to bulk promoted materials, as the alkali in these structures are highly mobile. Alkali can move easily in the tunnels or layers, segregate on the surface as well as desorb in high temperatures. Even so, the alkali are more stable than on surface promoted catalysts, as they are less likely to escape the structure and modify the supports properties from within, often leading to phases highly catalytically active in oxidation reactions.
This research was inspired by multiple aspects, such as: mechanistic significance (relation between composition-structure-reactivity, determining reaction mechanisms), civilizational significance (solving an ecological problem, improving the quality of life) and to produce a competitive catalyst for those presently used.
Despite common interest of the scientific community and intense research involving a wide spectrum of active phases, there is no satisfactory alternative to the expensive active phases used by industry. Such an alternative must be inexpensive, active and safe for the environment. Thus, transition metal oxides, promoted by alkali to increase catalytic activity, are prime candidates to replace the industrially used inert oxide supports decorated by noble metals. Among them, manganese oxides are often studied, as they are typically cheap, environmentally friendly and are catalytically active in numerous reactions. Their activity stems largely from the easy transition between oxidation states (from +2 to +7)74. The interest in these materials is very high, as can be seen by Fig. 7. Here, searches containing the word “manganese” in addition to either “soot combustion”
or “volatile organic compound oxidation” had the most results, closely followed by “noble metal” or “alkali”. The combination of “manganese” and “alkali” results, while the smallest, is also on the rise, showing the common interest in these materials as catalysts for pollutant removal.
Fig. 7 Amount of results after searching the scopus database for the depicted keywords as of 07.07.2019
Solving the problem of pollutant emission from combustion engines is of great importance to the development of civilization, as decreasing the release of soot
14 and VOCs will aid in avoiding many diseases affecting the population of large metropolises, increase the transparency of air and halt or even reverse adverse changes and contamination in ecosystems. A lack of definite and optimal solutions is in part due to the large variety of the forming pollutants. VOCs comprise a large group of forming volatile substances, while the composition of soot greatly depends on the conditions, in which it was formed. Thus, the aim is to find a universal catalyst for oxidation reactions, operating using a number of mechanisms (formation of reactive oxygen species, oxidation of NO to NO2), which will be thermally stable, active, inexpensive and safe for the environment.
3. Strategy of investigation
3.1. Soot and volatile organic compounds
The composition of soot can vary greatly depending on the source and prevailing conditions during its formation. This problem also exists for model soot, as it is necessary to maintain similar properties of the tested material across all studies. Model soot is used to achieve reproducible results in order to gather insight on how the soot combustion process itself occurs over the specific catalyst and allows the comparison of soot related studies among research groups.
One such model soot is Printex, which is obtained from the thermal decomposition of hydrocarbons under strictly controlled conditions. In the Printex model soot family there are three main soot types, which differ in composition and properties:
PrintexU, Printex80 and Printex85. According to the manufacturer they differ in average particle size (25, 15 and 16 nm) and specific surface area (100, 220, 200 m2/g, respectively) amongst other properties. They also differ in composition, with Printex80 containing less amorphic carbon and more graphitic carbon than the others, for example. These differences influence the temperature of combustion, as there is an 80°C difference in temperature at 50% combustion between them 75. Therefore, the most difficult to combust, Printex80, was chosen in this work to obtain the most active catalyst for the most incombustible soot.
Similarly to model soot, the choice of volatile organic compound to examine in regards to the reaction and conditions is crucial. Therefore, methane and propane were chosen as model VOCs, as both are among the basic building blocks at the start of soot and other VOC formation. Their polymerization leads to the formation of other VOCs and aromatics, which can escape into the environment and/or coalesce into the larger soot particles. Furthermore, methane and propane are both used as fuels in the transportation sector and it is necessary to ensure that the unburned fuels do not escape into the environment. Propane is the more traditional VOC of the two but also more easily combustible than methane, as it is more difficult to activate the more inert methane molecule.
Thus, an active catalyst for the oxidation of both methane and propane will aid in minimizing two of the most basic and common VOCs formed during the combustion process in engines.
Birnessite, a layered structure phyllomanganate, is one of the most commonly found forms of manganese oxides in nature (in soils, ore deposits, marine nodules, etc.) but can also be produced synthetically (through e.g. sol-gel, hydrothermal method) 74,76. The basic birnessite structure is triclinic and is comprised of edge sharing MnO6 octahedra, which form two dimensional layers (Fig. 8) 77. Therefore, it is sometimes referred to as an octahedral layered (OL) material. The interlayer space is occupied by water molecules and/or metal cations, from alkali cations to divalent second group and transition metals (Ca2+, Mg2+, Ni2+, Ba2+, Pb2+, Sr2+)78. The chemical formula is typically written as AMn4O8, with A denoting the intercalated cations. The charge of the interlayer cations is balanced by the decrease in manganese average oxidation state from 4 to typical values between 3.5 and 3.9, with manganese in tetravalent, trivalent and sometimes divalent oxidation states 74,79. When found in an aqueous environment, the layers of birnessite are known to exhibit an interlayer spacing of ~10 Å, which, upon drying in air at room temperature, decreases to ~7 Å. With the intercalation of larger cations, such as Ca2+, Mg2+ or Ni2+, the interlayer spacing of birnessite is known to remain at ~10 Å 79.
Fig. 8 Layered structure of birnessite, with intercalated cations located between layers of MnO6 octahedra
Birnessite is intensely studied by the scientific community for various applications and is a known catalyst in numerous reactions. It has been tested for application as cathodes for rechargeable lithium batteries, electrochemical capacitors, magnetic materials and as a sorbent material 80–83. Birnessite was found to be an active electrocatalyst in water oxidation, used for decomposition or degradation reactions of organics 84–86. Birnessite is also a highly active catalyst in VOC combustion for compounds such as: benzene, formaldehyde, acetone, methanol, 2-propanol 87–89. Likewise, its activity in soot oxidation has been confirmed repeatedly 90–92.
While birnessite is similar to phyllomanganates, cryptomelane is the analog of the natural mineral hollandite and is also one of the major manganese oxide minerals found in the deep-sea manganese nodules and in soil sediments 74,93,94. The cryptomelane structure is formed of, similarly to birnessite, MnO6 octahedral building blocks. The one dimensional tunnelled structure is formed by double- column walls of edge-sharing MnO6 chains, giving a tunnel dimension of 4.6 Å x 4.6 Å (Fig. 9) 95. The tunnels contain the intercalated cations, which stabilize the structure and are highly mobile due to their weak interaction with the surrounding manganese oxide. Due to the size of the tunnel, the intercalated cations are restricted largely to alkali, with the exception of caesium and francium.
Thus, the formula can be written as AxMn8O16 (A denotes the cations).
To compensate the charge, the average manganese oxidation state in cryptomelane is around 3.8, resulting from the prevalence of Mn4+, with small amounts of Mn3+ and Mn2+96.
Fig. 9 Tunnelled structure of cryptomelane, with intercalated cations located in tunnels of 2x2 wide columns of MnO6 octahedra
As the intercalated cations may be exchanged, cryptomelane is known as an octahedral molecular sieve (OMS-2). The high mobility of cations and the possibility of their exchange has led to many studies for the application of cryptomelane as molecular sieves or electrode materials for lithium batteries 97,98. OMS-2 has also been studied vigorously for use in catalysis, where the high activity is attributed to a highly porous structure, mild surface acid-base properties, ion exchange ability and facile lattice oxygen mobility 99. Cryptomelane has shown promise in degradation, decomposition and oxidative dehydrogenation reactions 93,94,100,101. Similarly to birnessite, cryptomelane is active in VOC combustion for compounds such as dimethyl ether, ethanol, ethyl acetate and toluene 70,71,99,102,103
. Cryptomelane is also an active catalyst for soot combustion 90.
3.4. Aim and research strategy
When released into the environment, both soot and volatile organic compounds can pose a serious health concern. The most promising way to minimize the amount of escaped pollutants from combustion engines is through the use of filters coated by catalytically active materials, which are meant to trap and combust the pollutants in the lowest possible temperatures through catalytic oxidation. The commonly used catalysts are effective but expensive, therefore alternative active phases are explored.
In this work the alkali nanostructured manganese oxide phases of birnessite and cryptomelane were proposed as cheap, efficient and environmentally friendly replacements for the expensive active phases used presently. The tunnelled cryptomelane and layered birnessite are widely known for their catalytic activity in oxidation reactions and their properties can be tuned through the intercalation of different cations or the dispersion of minimal amounts of noble metal nanoparticles on their surface.
The main aim of this work was the development of a universal catalyst for the oxidation of soot and volatile organic compounds based on manganese oxides nanostructured by alkali. This aim was achieved through the following tasks:
- Study of the most efficient way to increase the catalytic activity of manganese oxides for oxidation reactions by promoting them with alkali. The first goals of the work were to determine the most efficient way for promotion to maximize catalytic activity. The results clearly show alkali nanostructuration of manganese oxides to layered birnessite and tunnelled cryptomelane phases as the most beneficial.
- Study of the influence of the intercalated group I cation type (from H+ to Cs+) on the manganese oxide nanostructure. In order to determine the source of activity of an active phase, it is necessary to thoroughly characterize the material in regards to several key features, such as its composition, bulk structure, lattice oxygen mobility, specific surface area, electrodonor properties and surface morphology. A series of birnessite and cryptomelane phases containing different incorporated cations was prepared and characterized in order to showcase the most vital properties ruling high catalytic activity over nanostructured manganese oxides.
19 - Determining activity of the prepared phases in soot and VOC oxidation and the prevalent reaction mechanisms. The prepared catalysts were tested in oxidation reactions involving soot, propane and methane. Soot combustion was examined in 3 different contact modes: tight, loose and loose contact with NO addition, to determine the mechanism at work depending on soot/catalyst contact. Methane and propane were used as model volatile organic compounds, as they are difficult to oxidize and present alongside soot during the combustion of fuels. The thorough characterization of the materials revealed key correlations between activity, structure, composition and morphology, which were used to optimize the designed catalytic systems and maximize catalytic activity.
- Decoration of the most active birnessite and cryptomelane phases with noble metal nanoparticles. While birnessite and cryptomelane are known for high activity, the use of miniscule amounts of noble metal nanoparticles can be used to expand the range of oxidation reactions that the manganese supports are active in. The conditions in combustion engines and their exhaust are ever changing, thus a catalytic system must be robust and highly active no matter the reactant.
The measurable effect of the PhD project is the expanded knowledge concerning the properties (lattice oxygen and thermal stability, electrodonor properties) of manganese oxides nanostructured by alkali as well as the factors contributing to their high catalytic activity. Through thorough characterization using multiple techniques, the properties of the prepared materials were determined and used to reveal the prevalent mechanisms involved in soot and VOC oxidation.
4. Experimental Methods
Each prepared catalyst was subjected to thorough characterization to determine the elemental and phase composition, structural and morphological traits, the properties of the surface as well as the catalytic activity and stability.
This complete examination was the basis for the detailed findings presented in this work.
As the details of the applied experimental protocols are given in each appended Paper (Table 1) only the basic information or short description emphasizing the main reason, for which the method was used and what information was gathered, is provided below.
Table 1 Depiction of methods used in appended Papers
I II III IV V VI VII VIII
XRF x x x
XRD x x x x x x x x
RS x x x x x x x x
TEM x x x x x
BET x x x x
WF x x x x
TGA/DSC x x
TPO soot x x x x x x x
TPO VOC x x
As can be inferred from the table, the principal techniques in the PhD project were XRD and Raman Spectroscopy, TEM, work function determination and TPO.
This clearly indicates that most of the research was focused on phase characterization, imaging, determining the influence of alkali on the materials properties and determining catalytic activity, respectively. The presence of alkali creates the need for detailed documentation of the induced electronic changes, thus, apart from standard methods of catalyst characterization, the Kelvin
21 (work function determination) and Species Resolved-Thermal Alkali Desorption (alkali thermal desorption and stability) methods were employed. As these methods are not common, they have been described with more detail below.
4.1. Elemental composition
Verification of elemental composition is a crucial first step in the examination process, as it confirms the presence and quantity of desired elements and the lack of contaminants.
X-ray Fluorescence Spectroscopy (XRF)
X-ray fluorescence was the main technique employed to confirm elemental composition. Due to the high sampling depth, the result of the measurement is an averaged elemental composition of the sample in its complete volume.
The measured fluorescence radiation is characteristic of the excited element, which allows the qualitative identification of elements in a sample. Furthermore, based on the intensity of the measured peaks, with the appropriate calibration it is possible to determine the quantitative data concerning the sample composition. Due to the nature of the fluorescence, the method does not allow the quantitative determination of light elements (i.e. Li, C, O), but is very capable of determining the composition of transition metal oxide-based catalysts and their promoters (noble metals, alkali from Na to Cs). X-ray fluorescence was used to determine the composition of the studied active phases, with results of the tests included in Papers II, VI and VII.
4.2. Phase composition
Following elemental composition, phase composition aims at determining the crystal structure of the prepared materials, confirming successful synthesis.
The structure must be confirmed both in the bulk volume of the sample and on its surface, expelling doubts concerning the presence of impurities and shedding light on the cell parameters and particle sizes of the synthesized active phase.
X-ray Diffraction (XRD)
Powdered X-ray diffraction measurements were used to determine the structure and share of crystalline phases in the prepared active phases. In this work,